Influence of Storage Temperature on Orthodontic ElasticsCorrespondence Address :
Dr. R Piradhiba,
No.189A, A2. Hicon Villa, Kamaraj Salai, Kottivakkam, Chennai, Tamil Nadu, India.
Introduction: Orthodontic elastics are a very significant tool in orthodontics, as it is the most commonly used force delivering unit. Temperature plays a key role in the amount of force that elastics are able to produce. And, hence there is a need to evaluate the influence of storage temperature on the properties of orthodontic elastics before its clinical use.
Aim: The objective of this study was to evaluate the influence of different storage temperature of latex orthodontic elastics.
Materials and Methods: This cross-sectional study was conducted at Sathyabama Dental College and Hospital, Chennai, in November 2019. Sample of 40 latex orthodontic elastics (TP Orthodontics, medium force, standard size of 3/16'') were divided into four groups with 10 elastics each, based on their storage temperature and stored in closed plastic packages. Group 1 was kept as a Control group and Group 2, Group 3 and Group 4 were stored in three Incubators under the specified storage temperatures such as 26-28°C, 4-8°C, 37°C respectively. The elastics were stretched and their forces measured in six progressive increases of 100% of their inner diameter, starting at a level of 100% stretching, with the Universal Testing Machine, Instron. The samples were also tested for Maximum Stress (MPa), Maximum Force (N), Maximum Elongation (%) and Break Distance (mm). Data were analysed using SPSS software version 16.0, one-way analysis of variance (ANOVA) and post-hoc test.
Results: On evaluating the stress at 100%, 200%, 300%, 400%, 500%, 600% of strain, there was no statistically significant difference between the groups. Maximum Stress MPa was 26 found to be 24.12±3.32, 25.12±3.42, 23.3±3.41, 23.97±3.50 for group1, group 2, group 3 and group 4 respectively. Maximum Elongation (%) was found to be 1369.0±25.108, 1364.0±23.190, 1359.0±35.103, 1363.0±34.657 for group1, group 2, group 3 and group 4, respectively. Break Distance (mm) was found to be 68.48±1.267, 68.28±1.267, 67.87±1.77 and 68.19±1.727 for group1, group 2, group 3 and group 4, respectively. And none of the parameters tested showed statistical significance between the four groups.
Conclusion: Latex elastics may be stored under any of the conditions tested in the present study over a period of one month, since different storage temperatures over a period of one month did not interfere in their mechanical properties.
Break, Elongation, Stress, Strain
Date of Submission: Feb 08, 2021
Date of Peer Review: Mar 10, 2021
Date of Acceptance: May 25, 2021
Date of Publishing: Jul 01, 2021
• Financial or Other Competing Interests: None
• Was Ethics Committee Approval obtained for this study? Yes
• Was informed consent obtained from the subjects involved in the study? NA
• For any images presented appropriate consent has been obtained from the subjects. NA
PLAGIARISM CHECKING METHODS:
• Plagiarism X-checker: Feb 08, 2021
• Manual Googling: Feb 16, 2021
• iThenticate Software: May 05, 2021 (7%)
ETYMOLOGY: Author Origin
- Emerging Sources Citation Index (Web of Science, thomsonreuters)
- Index Copernicus ICV 2017: 134.54
- Academic Search Complete Database
- Directory of Open Access Journals (DOAJ)
- Google Scholar
- HINARI Access to Research in Health Programme
- Indian Science Abstracts (ISA)
- Journal seek Database
- Popline (reproductive health literature)